Temperature and carrier density-dependent spin dynamics for GaAs/AlGaAs quantum wells (QWs) with different structural symmetries have been studied by using time-resolved Kerr rotation technique. The spin relaxation time is measured to be much longer for the symmetrically designed GaAs QW comparing with the asymmetrical one, indicating the strong influence of Rashba spin-orbit coupling on spin relaxation. D'yakonov-Perel' mechanism has been revealed to be the dominant contribution for spin relaxation in GaAs/AlGaAs QWs. The spin relaxation time exhibits non-monotonic-dependent behavior on both temperature and photo-excited carrier density, revealing the important role of non-monotonic temperature and density dependence of electron-electron Coulomb scattering. Our experimental observations demonstrate good agreement with recently developed spin relaxation theory based on microscopic kinetic spin Bloch equation approach.
Spin dynamics and the related physics in semiconductors have drawn much attention in the past years because of its importance to realize novel spin-electronic devices . In recent years, electron spin relaxation in many types of materials, especially in low dimensional III-V group semiconductor heterostructures, has been studied extensively both theoretically and experimentally . The relevant spin relaxation mechanisms, such as the Elliott-Yafet, Bir-Aranov-Pikus (BAP), and D'yakonov-Perel' (DP) mechanisms as well as hyperfine interactions, have been well established to describe spin relaxation and dephasing dynamics. However, the relative importance of these mechanisms strongly depends on material design and temperature as well as carrier concentration and so on. Previous investigations in literature show that the BAP mechanism dominates the spin relaxation at low temperatures for bulk GaAs [2, 3] and GaAs/AlGaAs quantum wells (QWs) [4, 5], whereas DP mechanism dominates spin relaxation in other regimes. However, recent reexaminations using the microscopic kinetic spin Bloch equation approach [6–9] have revealed that the BAP mechanism is much less important than DP mechanism for intrinsic III-V group semiconductors, even at low temperatures. The DP mechanism resulting from spin-orbit coupling in systems lacking inversion symmetry, such as zinc-blende structure or asymmetric confining potentials in QWs, has a spin relaxation rate inversely related to the momentum scattering rate . Electron spin relaxation in GaAs QWs has been experimentally studied through temperature [10, 11] and QW width dependence [10–12], and DP mechanism has been revealed to dominate spin relaxation in intrinsic QWs at high temperatures . The oscillatory spin dynamics study for two-dimensional electron gas (2DEG) at low temperatures also demonstrated the dominance of DP mechanism in the weak momentum scattering regime . The observed enhancement of spin relaxation time resulting from electron-electron scattering in n-doped GaAs/AlGaAs QW agrees with DP mechanism governed by electron-electron scattering as well [14–17]. The experimental observation of electron spin relaxation time maximum for temperature-dependent study in a high-mobility GaAs/AlGaAs 2DEG has also revealed the importance of electron-electron Coulomb scattering .
The spin-orbit (SO) coupling leads to a strong momentum-dependent mixing of spin and orbital-momentum eigenstates, so that scattering processes change spin and orbital angular momentum, and therefore contribute to spin relaxation accordingly [19–21]. For electrons in two-dimensional semiconductor heterostructures or QWs, the Rashba SO coupling due to structure inversion asymmetry and the Dresselhaus SO coupling due to bulk inversion asymmetry in the compounds cause electron spin relaxation and decoherence through spin precession of carriers with finite crystal momentum k in the effective k-dependent crystal magnetic field of an inversion-asymmetric material. Therefore, spin relaxation and decoherence studies in semiconductors have revealed important physics of SO coupling. Since carrier spin relaxation is related to several competing mechanisms and particularly different materials and structural designs, different SO coupling is involved to spin relaxation processes. Thus, the experimental investigation of spin relaxation and its dependence on temperature and carrier density have been found to vary widely between different samples. In this study, we have designed two GaAs/AlGaAs QWs with different structural symmetries. The spin relaxation time is measured to be much shorter for the asymmetrically designed GaAs/AlGaAs QW comparing with the symmetrical one, indicating the strong effect of Rashba SO coupling on spin relaxation. The comprehensive studies of temperature and carrier density dependence of spin relaxation time for both samples have revealed that electron spin relaxation in GaAs/AlGaAs QWs is governed mainly by DP mechanism in the entire temperature regime. The spin relaxation time exhibits non-monotonic behavior for both temperature and photo-excited carrier density dependence, revealing the important role of non-monotonic temperature and density dependence of electron-electron Coulomb scattering. Our experimental observations demonstrate good agreement with recently developed spin relaxation theory based on microscopic kinetic spin Bloch equation approach [6–9].
The samples used in our experiments were n-modulation-doped single GaAs/AlGaAs QW with well width of 10 nm grown by molecular beam epitaxy on (100)-oriented semi-insulating GaAs substrates. As shown in Figure 1, one of the samples is designed to be symmetric with two-side symmetric Al0.3Ga0.7As barriers and δ-doping concentration of 2 × 1010 cm-2. The other sample is designed to be asymmetric with different aluminum components at two sides (Al0.3Ga0.7As for the upside barrier and Al0.25Ga0.75As for the downside barrier) and asymmetric doping concentration as well (the nominal upside n-modulation doping is 2 × 1011 cm-2 and the downside doping is 2 × 1010 cm-2). The rest layer structures and growth conditions are identical for two samples.
In our time-resolved magneto-Kerr rotation measurement, a Ti:Sapphire laser system (Chameleon Ultra II, Coherent Inc., USA) provided 150 fs pulses with repetition rate of 80 MHz. The pump beam with central wavelength ranging from 770 to 860 nm was incident normal to the sample, while probe beam was at an angle of about 30° to the surface normal. The polarization of the pump beam was adjusted to be circularly polarized and the probe beam was linearly polarized. The sample was mounted within a Janis closed-cycle optical cryostat, which is located in-between two poles of an electromagnet. After reflection from sample, the Kerr rotation signal was detected by a sensitive optical bridge and lock-in amplifier. The photoluminescence (PL) measurements have been first performed at wide temperature range to check the sample's quality and identify the band-edge energies for the specially designed samples.
Results and discussion
Both samples have shown very good PL response up to room temperature as shown in Figure 2, indicating a good sample quality. The PL peak at 848 nm is related to the band edge of QW and the peak at 870 nm is related to the band edge of GaAs substrate. The band edge-related PL peak for QW has blue-shifted to 798 nm at 10 K as expected. The time-resolved Kerr rotation measurements are then performed at different temperatures and photo-excitation powers with excitation wavelength centered either at the resonant position of the band edge PL peak of QWs or well above it. The typical time-resolved Kerr rotation signals measured at 20, 200, and 250 K with an excitation wavelength of 798 nm and pumping electron densities of 1.15 × 1011 cm-2 for the asymmetric GaAs QW have been presented in Figure 3a. The temperature dependence of electron spin relaxation times extracted from the exponential decay function fitting of time-resolved Kerr response for both symmetric and asymmetric GaAs/AlGaAs QWs is shown in Figure 3b. The measured spin relaxation time for the symmetric GaAs/AlGaAs QW is in general longer than the asymmetric one at low temperature regime (< 100 K). This result is consistent with the well-established DP spin relaxation mechanism, in which the SO coupling plays an important role for electron spin relaxation. It is naturally expected that the Rashba SO coupling in the asymmetric sample should be stronger than the symmetric one, whereas the Dresselhaus SO coupling could be similar for two samples. The shorter spin relaxation time for the asymmetric QW is caused by much stronger inhomogeneous magnetic fluctuations resulting from stronger Rashba SO coupling than the symmetric QW. Meanwhile, electron spin relaxation times for both symmetric and asymmetric GaAs/AlGaAs QWs have shown non-monotonical dependence on temperature. Spin relaxation time increases first with increasing temperature, showing a peak value of 399 ps around 180 K, and then decreases with further increase in temperature for the asymmetric QW. The symmetric GaAs/Al0.3Ga0.7As QW shows the similar temperature-dependent spin relaxation time behavior, but with a maximum spin relaxation time of 592 ps observed around 60 K. The BAP mechanism, in which the spin relaxation is caused by spin-flip via the electron-hole exchange interaction, predicts that the spin-relaxation time decreases rapidly with increasing temperature in low-temperature regime. However, the observed low temperature dependence of spin relaxation is in contrast to the BAP mechanism. Rather, the appearance of a peak in the temperature-dependent spin relaxation time for both symmetric and asymmetric GaAs QW structures agrees well with the theoretical reexamination of spin dynamics in both QW and bulk intrinsic III-V group semiconductors [6–9], in which BAP mechanism has been shown to be much less important than DP mechanism, even at low temperatures. The strengthening momentum scatterings at higher temperatures suppress the inhomogeneous broadening (the random spin precession), and tend to prolong the spin relaxation time with DP mechanism, in which spin relaxation time is inversely proportional to the momentum scattering time τ p The appearance of the peaks in Figure 3b originates from the DP mechanism controlled by electron-electron Coulomb scattering. In addition, as discussed in references [6–9], electron-electron Coulomb scattering rate is a non-monotonic function of temperature and electron density with a minimum of corresponding to the crossover from the degenerate limit to the non-degenerate one at Fermi temperature T F = E F /K B[6–9].
When temperature further increases, electron-phonon scattering will then strengthen and become comparable to electron-electron scattering, eventually dominate the spin relaxation process; thus, spin relaxation time decreases with further rising temperatures. As a result, spin relaxation time shows a maximum. Considering the total electron density, n e is the sum of optically excited carrier density and doping density (assuming fully ionized Si doping), the peak of temperature-dependent spin relaxation time is calculated to appear at about 59 and 140 K for the symmetric and asymmetric GaAs/AlGaAs QW samples under optically pumped electron density of 1.15 × 1011 cm-2, respectively. This, however, only agrees with the observed peak position for the symmetric sample. The inconsistence for the asymmetric sample may result from the uncertainty of the actual electron density.
The typical time-resolved Kerr rotation signals measured at 10 K with the excitation wavelength of 798 nm at three different pumping electron densities for the asymmetric GaAs QW have been presented in Figure 4a. The optically pumped electron density dependence of electron spin relaxation times measured at 10 K with the excitation wavelength of 798 nm for both symmetric and asymmetric GaAs/AlGaAs QWs is shown in Figure 4b. Again, the electron spin relaxation times for both symmetric and asymmetric GaAs/AlGaAs QWs have shown non-monotonic dependence on excitation density with a peak appearing at electron density of n c = 1.5-1.7 × 1011cm-2 The non-monotonic density dependence of spin relaxation time mainly results from electron-electron Coulomb scatterings contribution at low temperature. It is known that, in the strong scattering regime, the spin relaxation time can be expressed as [6–9], where 〈Ω⊥ 2〉 is the average square of the component for precession vector in the plane perpendicular to i, and is the momentum scattering time. In the non-degenerate (low density) regime, the electron-electron scattering increases with electron density, whereas the inhomogeneous broadening barely changes since the distribution function is close to the Boltzmann distribution. The spin relaxation is thus governed by strengthening electron-electron scattering with increasing carrier density. Therefore, spin relaxation time increases with increasing excitation density. In degenerate (high density) regime, both and the inhomogeneous broadening 〈Ω⊥ 2〉 increase with electron density, leading to the decreased spin relaxation time with carrier density. The similar non-monotonic-dependent behavior on excitation density for spin relaxation time has also been experimentally observed for intrinsic GaAs QW  and bulk CdTe crystal [23, 24] at room temperature. DP mechanism has been revealed to dominate the electron spin relaxation at room temperature. The doping density-dependent electron spin relaxation investigation at low temperature for n-type bulk GaAs has also observed a peak in spin-dephasing times , and this peak has been attributed to the influence of electron screening and scattering on the spin dynamics of the excited electrons [25, 26]. The high temperature regime (280-400 K) investigation of spin relaxation time as a function of carrier density for bulk GaAs also confirmed the dominance of DP and electron optical-phonon scattering mechanism . Our experimental investigations for temperature and carrier density-dependent electron spin dynamics give further demonstration of DP mechanism-governed spin relaxation process in n-modulation-doped GaAs QWs.
In conclusion, the temperature and carrier density-dependent studies of spin relaxation time for modulation-doped GaAs/AlGaAs QWs have demonstrated a good agreement with recently developed spin relaxation theory based on microscopic kinetic spin Bloch equation approach. The spin relaxation time is measured to be much longer for the symmetrically designed GaAs QW comparing with the asymmetrical one, indicating the strong influence of Rashba SO coupling on spin relaxation. DP mechanism has been revealed to dominate spin relaxation for n-modulation-doped GaAs QWs in the entire temperature regime. Our experimental results provide further fundamental understanding of spin dynamics in modulation-doped heterostructures toward potential semiconductor spintronics application based on GaAs/AlGaAs material systems.
two-dimensional electron gas.
Dyakonov MI: Spin Physics in Semiconductors. Berlin: Springer-Verlag; 2008.
Lai TS, Liu XD, Xu HH, Jiao ZX, Wen JH, Lin WZ: Temperature dependence of electron-spin coherence in intrinsic bulk GaAs. Appl Phys Lett 2006, 88: 192106. 10.1063/1.2202754
Amo A, Viña L, Lugli P, Tejedor C, Toropov AI, Zhuravlev KS: Pauli blockade of the electron spin flip in bulk GaAs. Phys Rev B 2007, 75: 085202. 10.1103/PhysRevB.75.085202
Wagner J, Schneider H, Richards D, Fischer A, Ploog K: Observation of extremely long electron-spin-relaxation times in p-type delta-doped GaAs/Al x Ga 1-x As double heterostructures. Phys Rev B 1993, 47: 4786. 10.1103/PhysRevB.47.4786
Gotoh H, Ando H, Sogawa T, Kamada H, Kagawa T, Iwamura H: Effect of electron-hole interaction on electron spin relaxation in GaAs/AlGaAs quantum wells at room temperature. J Appl Phys 2000, 87: 3394. 10.1063/1.372356
Zhou J, Wu MW: Spin relaxation due to the Bir-Aronov-Pikus mechanism in intrinsic and p-type GaAs quantum wells from a fully microscopic approach. Phys Rev B 2008, 77: 075318. 10.1103/PhysRevB.77.075318
Jiang JH, Wu MW: Electron-spin relaxation in bulk III-V semiconductors from a fully microscopic kinetic spin Bloch equation approach. Phys Rev B 2009, 79: 125206. 10.1103/PhysRevB.79.125206
Jiang JH, Cheng JL, Wu MW: Spin relaxation in n -type GaAs quantum wells from a fully microscopic approach. Phys Rev B 2007, 75: 045305. 10.1103/PhysRevB.75.045305
Wu MW, Jiang JH, Weng MQ: Spin dynamics in semiconductors. Phys Rep 2010, 493: 61. 10.1016/j.physrep.2010.04.002
Malinowski A, Britton RS, Grevatt T, Harley RT, Ritchie DA, Simmons MY: Spin relaxation in GaAs/Al x Ga 1-x As quantum wells. Phys Rev B 2000, 62: 13034. 10.1103/PhysRevB.62.13034
Ohno Y, Terauchi R, Adachi T, Matsukura F, Ohno H: Spin relaxation in GaAs (110) quantum wells. Phys Rev Lett 1999, 83: 4196. 10.1103/PhysRevLett.83.4196
Britton RS, Grevatt T, Malinowski A, Harley RT, Perozzo P, Cameron AR, Miller A: Room temperature spin relaxation in GaAs/AlGaAs multiple quantum wells. Appl Phys Lett 1998, 73: 2140. 10.1063/1.122403
Leyland WJH, Harley RT, Henini M, Shields AJ, Farrer I, Ritchie DA: Oscillatory Dyakonov-Perel spin dynamics in two-dimensional electron gases. Phys Rev B 2007, 76: 195305. 10.1103/PhysRevB.76.195305
Leyland WJH, John GH, Harley RT, Glazov MM, Ivchenko EL, Ritchie DA, Farrer I, Shields AJ, Henini M: Enhanced spin-relaxation time due to electron-electron scattering in semiconductor quantum wells. Phys Rev B 2007, 75: 165309. 10.1103/PhysRevB.75.165309
Wu MW, Ning CZ: A novel mechanism for spin dephasing due to spin-conserving scatterings. Eur Phys J B 2000, 18: 373. 10.1007/s100510070021
Wu MW, Metiu H: Kinetics of spin coherence of electrons in an undoped semiconductor quantum well. Phys Rev B 2000, 61: 2945. 10.1103/PhysRevB.61.2945
Wu MW: Spin dephasing induced by inhomogeneous broadening in D'yakonov-Perel' effect in a n -doped GaAs quantum well. J Phys Soc Jpn 2001, 70: 2195. 10.1143/JPSJ.70.2195
Ruan XZ, Luo HH, Yang J, Xu ZY, Umansky V: Effect of electron-electron scattering on spin dephasing in a high-mobility low-density two-dimensional electron gas. Phys Rev B 2008, 77: 193307. 10.1103/PhysRevB.77.193307
Sham LJ: Spin relaxation in semiconductor quantum wells. J Phys Condens Matter 1993, 5: A51. 10.1088/0953-8984/5/33A/005
Averkiev NS, Golub LE, Willander M: Spin relaxation anisotropy in two-dimensional semiconductor systems. J Phys Condens Matter 2002, 14: R271. 10.1088/0953-8984/14/12/202
Pikus GE, Titkov AN: Optical Orientation. Edited by: Meier F, Zakharchenya BP. Amsterdam: North-Holland; 1984:73–131.
Teng LH, Zhang P, Lai TS, Wu MW: Density dependence of spin relaxation in GaAs quantum well at room temperature. EuroPhys Lett 2008, 84: 27006. 10.1209/0295-5075/84/27006
Ma H, Jin ZM, Ma GH, Liu WM, Tang SH: Photon energy and carrier density dependence of spin dynamics in bulk CdTe crystal at room temperature. Appl Phys Lett 2009, 94: 241112. 10.1063/1.3155428
Jiang JH, Wu MW: Comment on "Photon energy and carrier density dependence of spin dynamics in bulk CdTe crystal at room temperature". Appl Phys Lett 2010, 96: 136101. 10.1063/1.3371817
Krauß M, Schneider HC, Bratschitsch R, Chen Z, Cundiff ST: Ultrafast spin dynamics in optically excited bulk GaAs at low temperatures. Phys Rev B 2010, 81: 035213.
Shen K: A Peak in Density Dependence of Electron Spin Relaxation Time in n -Type Bulk GaAs in the Metallic Regime. Chin Phys Lett 2009, 26: 067201. 10.1088/0256-307X/26/6/067201
Oertel S, Hübner J, Oestreich M: High temperature electron spin relaxation in bulk GaAs. Appl Phys Lett 2008, 93: 132112. 10.1063/1.2993344
This study was supported by the National Basic Research Program of China under Grant Nos. 2011CB922200 and 2007CB924904; the National Natural Science Foundation of China under Grant Nos. 10974195 and 10734060.
The authors declare that they have no competing interests.
LFH carried out the time resolved Kerr rotation measurements for all samples and performed the calculation and analysis. YGZ helped out the experimental setup and instructions. XHZ conceived of the study and participated in its design and coordination as well as manuscript drafting. P H Tan performed the PL measurement. HQN and ZCN grew GaAs QW samples with high quality by molecular beam epitaxy method. All authors read and approved the final manuscript.
About this article
Cite this article
Han, L., Zhu, Y., Zhang, X. et al. Temperature and electron density dependence of spin relaxation in GaAs/AlGaAs quantum well. Nanoscale Res Lett 6, 84 (2011). https://doi.org/10.1186/1556-276X-6-84
- Spin Relaxation
- Spin Dynamic
- Spin Relaxation Time
- Bulk GaAs